Comprehensive study of carbon dioxide adsorption in the metal‒organic frameworks M2(dobdc) (M = Mg, Mn, Fe, Co, Ni, Cu, Zn)
Queen, Wendy L.; Hudson, Matthew R.; Bloch, Eric D.; Mason, Jarad A.; Gonzalez, Miguel I.; Lee, Jason S.; Gygi, David; Howe, Joshua D.; Lee, Kyuho; Darwish, Tamim A.; James, Michael; Peterson, Vanessa K.; Teat, Simon J.; Smit, Berend; Neaton, Jeffrey B.; Long, Jeffrey R.; Brown, Craig M.; Chem. Sci. 5 (2014) 4569–; doi:10.1039/C4SC02064B

data_1517477
_publ_section_title
;
 Comprehensive study of carbon dioxide adsorption in the metal--organic
 frameworks M2(dobdc) (M = Mg, Mn, Fe, Co, Ni, Cu, Zn)
;
_journal_issue                   12
_journal_name_full               'Chem. Sci.'
_journal_page_first              4569
_journal_paper_doi               10.1039/C4SC02064B
_journal_volume                  5
_journal_year                    2014
_chemical_formula_sum            'C5.5 H Co O6.01'
_chemical_formula_weight         222.14
_chemical_name_systematic        ' ?'
_space_group_IT_number           148
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_audit_creation_date             2014-01-17T16:02
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2014-01-17T16:02  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            18
_cell_length_a                   25.8735(12)
_cell_length_b                   25.8735
_cell_length_c                   6.8486(4)
_cell_measurement_temperature    10
_cell_volume                     3970.5(3)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      10
_diffrn_measurement_device_type  BT1
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     2.0785
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_exptl_crystal_colour            purple
_pd_block_id                     2014-01-17T16:02|1P5CO2_CO||bt1
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        166.25
_pd_meas_2theta_range_min        1.5
_pd_meas_number_of_points        3296
_pd_phase_name
'from /data/people/craigy/MgMOF/BT1/1108/MOF74.xtl'
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        166.2756
_pd_proc_2theta_range_min        1.5256
_pd_proc_info_datetime           2014-01-17T16:02:56
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 12 terms.
 Shifted Chebyshev function of 1st kind
      1:    724.040     2:   -52.4787     3:    139.403     4:    70.1875    
      5:    65.1653     6:    26.7079     7:    31.9387     8:    9.09212    
      9:    10.1339    10:   -4.15328    11:   -5.47016    12:    4.27962    
;
_pd_proc_ls_peak_cutoff          0.00500
_pd_proc_ls_profile_function
;
 CW Profile function number 3 with  19 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 Peak tails are ignored  where the intensity is below 0.0050 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0290
_pd_proc_ls_prof_wR_expected     0.0363
_pd_proc_ls_prof_wR_factor       0.0355
_pd_proc_number_of_points        3296
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   0.99
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     70
_refine_ls_number_restraints     5
_refine_ls_R_Fsqd_factor         0.09834
_refine_ls_shift/su_max          0.03
_refine_ls_shift/su_mean         0.01
_reflns_d_resolution_high        1.051
_reflns_d_resolution_low         12.937
_reflns_limit_h_max              24
_reflns_limit_h_min              0
_reflns_limit_k_max              12
_reflns_limit_k_min              -11
_reflns_limit_l_max              6
_reflns_limit_l_min              -6
_reflns_number_total             805
_cod_data_source_file            c4sc02064b2.cif
_cod_data_source_block           1P5CO2_CO_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (36
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (27
times).

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 1517465--1517482.cif.
;
_cod_original_cell_volume        3970.5(4)
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'C5.50 H Co O6.01'
_cod_database_code               1517477
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000